natural dye sensitizer in dye sensitized solar cell
Post on 28-Jan-2017
Embed Size (px)
Sains Malaysiana 45(8)(2016): 12271234
Natural Dye Sensitizer in Dye Sensitized Solar Cell (Pemeka Pewarna Semula Jadi dalam Pekaan Pewarna Sel Suria)
NURAIN NAJIHAH ALIAS* & KHATIJAH AISHA YAACOB
Blue-pea flower, turmeric, mulberries, brown rice, purple cabbage and Indian mulberry leave were successfully form on TiO2 mesoporous film using immersion method to produce TiO2 mesoporous photoanode for natural dye sensitized solar cells (DSSCs) assembly. The TiO2 mesoporous films were formed after calcinations at 450C for 30 min. The photoanodes were dipped in different types of natural dye for 24, 72 and 120 h. The properties of natural dye were investigated by ultraviolet-visible spectroscopy (UV-vis) and Fourier transform infrared spectroscopy (FTIR). From UV-Vis spectroscopy analysis, the wavelength range of the natural dye studied in this research lays between 350 and 800 nm. The FTIR result of the natural dye shows the present of intermolecular H-bond, C=O stretching vibration, C-O-C stretching vibration, C=C bending and C-H bending which was due to the component of anthocyanin, carotenoids and chlorophyll. The characterization including field emission scanning electron microscopy (FESEM), energy dispersive x-ray (EDX) and x-ray diffraction (XRD) were carried out on the TiO2 mesoporous film. On the other hand, the conductivity of electrolyte for liquid electrolyte, gel electrolyte and solid electrolyte were also investigated. Gel electrolyte has the highest conductivity, 26.1 mS/cm while liquid electrolyte and solid electrolyte obtained 17.34 and 0.45 mS/cm, respectively. Finally, solar cells were prepared by sandwiching the TiO2 mesoporous photoanode with Platinum (Pt) counter electrode. The results showed short circuit current, open circuit current voltage, fill factor and efficiency for all samples during the present of light. The highest efficiency was obtained from Blue-pea sample that immersed for 120 h with 0.123% efficiency.
Keywords: DSSCs; natural dye sensitized solar cells; solar energy
Bunga telang, kunyit, malberi, beras perang, kubis ungu dan daun mengkudu telah melekat pada lapisan TiO2 berliang meso dengan menggunakan kaedah rendaman bagi menghasilkan TiO2 berliang meso sebagai fotoanod untuk pewarna semula jadi sebagai pemeka dalam pewarna sel solar berkepekaan (DSSCs). Lapisan TiO2 berliang meso terbentuk selepas pengkalsinan pada suhu 450C selama 30 min. Fotoanod dicelup dalam pewarna semula jadi selama 24, 72 dan 120 jam. Sifat pewarna semula jadi telah dicirikan oleh Ultra Violet Visible Spektrofotometer (UV-vis) dan spektroskopi Fourier infra merah (FTIR). Melalui UV-Vis spektroskopi, gelombang pewarna semula jadi yang diperoleh adalah antara 350 dan 800 nm. Hasil FTIR pewarna semula jadi menunjukkan terdapat ikatan H, C=O, C-O-C, C=C dan C-H yang disebabkan oleh komponen daripada pada antosianin, karotenoid dan klorofil. Medan pancaran mikroskop elektron imbasan (FESEM), tenaga serakan sinar-x (EDX) dan pembelauan sinar-x (XRD) telah dijalankan ke atas lapisan TiO2 berliang meso. Konduktiviti elektrolit cecair, elektrolit gel dan elektrolit pepejal juga telah dikaji. Elektrolit gel mencatat konduktiviti tertinggi, 26.1 mS/cm manakala elektrolit cecair dan elektrolit pepejal memperoleh 17.34 dan 0.45 mS/cm. Fotoanod TiO2 berliang meso dicantum dengan elektrod kaunter Platinum (Pt). Nilai yang ditunjukkan adalah semasa litar pintas, voltan litar terbuka, faktor pengisian dan peratus keberkesanan untuk semua sampel. Bunga telang yang telah direndam selama 120 jam telah mencatat peratus keberkesanan yang tertinggi iaitu 0.123%.
Kata kunci: DSSCs; pewarna semula jadi sel solar berkepekaan; tenaga solar
The history of the sensitization of semiconductors to light of wavelength longer than that corresponding to the band gap has been presented elsewhere (Kim et al. 2011). Dye-sensitized solar cells or DSSCs use a process similar to photosynthesis to produce electrical energy. Dye-sensitized solar cells are a promising technology because they are inexpensive and resilient, making them ideal for large scale and small scale applications. However, they have lower efficiencies than most other types of solar cells, so
they require more space than other types of solar cells to produce the same amount of electric energy. Today, most solar cells manufactured in the world are silicon solar cells. There are several types of silicon solar cells, one of which are bulk silicon solar cells and thin-film solar cells. One of the next-generation solar cells expected to satisfy these demands is dye-sensitized solar cells. Grtzel (2013) reported high-efficiency cells using nanoporous titanium oxide semiconductor electrodes, ruthenium (Ru) metal complex dyes and iodine electrolyte solutions in
the journal of Nature in 1991. Since then, many studies have been actively carried out on DSSCs and showed their performance comparable to amorphous silicon thin films. These DSSCs have the advantages of low cost, lightweight and easy fabrication, but issues include durability and further improvement of their properties. In order to respond to these issues, many attempts have been made, such as solidifying electrolytes and improving materials and structures, but there have been no great breakthroughs yet. Dye-sensitized solar cells consist of dye-adsorbed porous TiO2 layer on fluorine doped tin oxide (FTO) glass as working electrode. Under the illumination of solar light, dye molecules are excited and electrons were produced. In order to generate meaningful electrical power from DSSCs, the electrons need to pass four important interfaces of DSSCs: dye/ TiO2, TiO2/FTO, electrolyte/counter electrode and dye/electrolyte. The nanoporous nature of the TiO2 layer provides high surface area that is great importance to the efficient photon-to-electricity conversion because it enhances dye loading and solar light absorption (Indriana Kartini et al. 2001). However, it also provide abundant TiO2 surface site (direct route) and bare FTO conducting site (indirect route), where the photo-injected electrons may recombine with electrolyte. The recombination will cause the loss of the photocurrent. So the photovoltaic performance of DSSCs was seriously decreased (Cameron & Peter 2003). The introduction of a compact layer between the interfaces of the FTO/porous TiO2 has been proven theoretically and practically effective to block the electrons recombination via the indirect route as shown in Figure 1 (Haque et al. 2004; Nakade et al. 2004, Zhu et al. 2006). Efficiencies over 10% have been achieved (Grtzel 2013). Therefore, the natural dye as sensitizer in dye sensitized solar cell is introduced. Metal-free dyes such as derivatives (Li et al. 2006), coumarin dye (Hara et al. 2001), porphyrin dyes (Tokuhisa & Hammond 2003) and cyanine and merocyanine dye (Kazuhiro Sayamaa, 2003) have been used as sensitizers, but did not achieve the same solar conversion efficiency as ruthenium dyes. In this research, blue-pea flower, turmeric, mulberries, brown rice, purple cabbage and Indian mulberry leave were used and successfully form on TiO2 mesoporous film using immersion method in order to produce photoanode for natural dye sensitized solar cells (DSSCs). The highest efficiency achieved in this work was 0.123% which was higher than reported value for ruthenium dyes. In addition this dye has the advantage which can be produced at low cost, as it does not contain the rare metal ruthenium and easy to synthesize.
In this research, fluorine tin oxide (FTO) with sheet resistance ~7 /square was used as substrates. The FTO substrates were cleaned with distilled water and soap
(Extran) and then rinse with distilled water and sonicated for 15 min. The TiO2 mesoporous photoanodes were selected as the working electrode due to exhibited best operating performance in classical DSSCs. In this research the TiO2 mesoporous layer was deposited by doctor blade using commercialised Dyesol paste 18NR-T. The substrates were then sintered at 450C in the Lenton furnace in order to achieve good contact between FTO and TiO2 nanoparticles.
PREPARATION OF NATURAL DYE SENSITIZERS
The blue-pea flower, turmeric, mulberries, purple cabbage and Indian mulberry leave were cut into small pieces. Each natural dye sources were weight for 50 g and soak with 124 mL of ethanol and boil for 30 min. The beaker should be cover with aluminium foil or plastic sheet in order to prevent ethanol from evaporate. Then, the solutions were cool to room temperature for 24 h. After that, by using filter funnel and conical flask, the solution was filtered in order to remove solid fragments. The extract solution of all natural dyes (Figure 2) will appear, for blue-pea flower it has absolutely blue colour of solution. The solution was then kept in the amber bottle to avoid the solution from direct sunlight. After the filtration process, the FTO substrates with TiO2 transparent layer were dipped in natural dye solution for 24, 72 and 120 h. However, for brown rice, there was no need to boil the mixture of brown rice with ethanol. First, the brown rice was weight for 50 g. Then, it was cleaned with distilled water. Let it dry in room temperature for one day. Next, soak together the 50 g brown rice with 124 mL of ethanol in beaker for 48 h with the ratio of 1:1. After that, filter the solution using the filter funnel and conical flask. The filter paper used is Grade 4 which is for rapid filtering with excellent retention of coarse particles. The filtration process was done in the fume cupboard. After the filtration process, FTO glasses that deposited with TiO2 were dipped in the solution for 24, 72 and 120 h. The beaker must be properly stored and protected from direct sunlight.